Jones, David, Rongzong Wu, John T. Harvey (2008) Reflective Cracking Study: First-level Report on HVS Testing on Section 591RF - 45 mm MAC15TR-GOverlay. Institute of Transportation Studies, University of California, Davis, Research Report UCPRC-RR-2007-04
experiment being performed at the Richmond Field Station (RFS) to validate Caltrans overlay strategies for the
rehabilitation of cracked asphalt concrete. It describes the results of the sixth HVS reflective cracking testing
section, designated 591RF, carried out on a 45-mm half-thickness MAC15TR gap-graded overlay with 15 percent
recycled tire rubber. The test forms part of Partnered Pavement Research Center Strategic Plan Element 4.10:
“Development of Improved Rehabilitation Designs for Reflective Cracking.”
HVS trafficking on the section commenced on January 10, 2007, and was completed on June 25, 2007. A total of
2,554,335 load repetitions, equating to 90.8 million ESALs and a Traffic Index of 15.4, was applied during this
period. Temperatures were maintained at 20°C±4°C for the first one million repetitions, then at 15°C±4°C for the
remainder of the test. Caltrans and the UCPRC jointly agreed to halt HVS trafficking at this point as there was no
indication of the failure criteria being reached in the near future. Findings and observations based on the data
collected during this HVS study include:
• No cracking was observed on the section. This implies that the MAC15TR overlay successfully prevented
• The average deformation and average maximum rut depth across the entire test section was just 1.7 mm and
4.6 mm, respectively, considerably lower than the failure criterion of 12.5 mm. The maximum rut depth
measured was 8.2 mm. The MAC15TR overlay thus did not appear susceptible to rutting at the temperature
range under which the test was conducted.
• Ratios of final-to-initial elastic surface deflections under a 60 kN wheel load increased by between 3.7 and 4.0
times along the length of the section. The ratios for in-depth deflections show that damage increased at all
depths in the pavement structure by the end of trafficking. Loss of stiffness was highest in the area of most
severe cracking in the underlying DGAC layer.
• Analysis of surface profile and in-depth permanent deformation measurements indicates that most of the
permanent deformation (55 and 60 percent) occurred in the asphalt-bound surfacing layers (overlay and
cracked DGAC) with the remainder mostly in the aggregate base layer.
No recommendations as to the use of the modified binders in overlay mixes are made at this time. These
recommendations will be included in the second-level analysis report, which will be prepared and submitted on
completion of all HVS and laboratory testing.